# Coupling local and non-local damage evolutions with the Thick Level Set model

- Nicolas Moës
^{1}Email author, - Claude Stolz
^{1, 2}and - Nicolas Chevaugeon
^{1}

**1**:16

https://doi.org/10.1186/s40323-014-0016-2

© Moës et al.; licensee Springer. 2014

**Received: **25 April 2014

**Accepted: **9 September 2014

**Published: **15 October 2014

## Abstract

### Background

The Thick Level Set model (TLS) is a recent method to delocalize local constitutive models suffering spurious localization. It has two major advantages compared to other delocalization methods. The first one is that the transition from localization to fracture is taken into account in the model. The second one is that the delocalization only acts when and where needed. In other words, the TLS has no effect when the local model is stable. The former advantage was already detailed in several papers (IJNME 86:358-380, 2011, CMAME 233:11-27, 2012, IJF 174:49-60, 2012). This paper concentrates on the latter advantage.

### Methods

The TLS delocalization approach is formulated as a bound on the damage gradient. The non-local zone is defined as the zone where the bound is met whereas the local zone is defined as the zone where it is not met. The boundary (localization front) between the local and non-local zone is the main unknown in the problem.

### Results

Based on the new model, a 1D pull-out test is solved both analytically and numerically. Different regimes are observed in the solution as the loading progresses: fully elastic, local damage, coupled local/non-local damage and, finally, purely non-local damage.

### Conclusions

The new model introduces delocalization as an inequality allowing local damage to develop in zones whereas non-local damage may develop in other zones. This reduces dramatically the cost of implementation of such models compared to fully non-local models.

### Keywords

Damage Delocalization Non-local damage models Level set TLS## Background

Although the scope of TLS application is much wider, we consider in this paper the fracture of quasi-brittle structures under quasi-static loading and under small deformation assumption. The loading is proportional to a scalar parameter. The material is modelled by a time-independent elasto-damage constitutive model with scalar damage. Due to quasi-static analysis, the loading parameter must be controlled especially when bifurcation occurs.

The TLS model was introduced in several papers [1],[2] and [3],[4]. It lies between continuum damage mechanics and fracture mechanics. Indeed, crack opening is allowed across fully damaged zones (see [2] for instance). The fully damaged zone is located by a level set. Let us note that the description above is different from a diffuse vision of the crack in which crack opening is not explicitly modeled as in the phase-field approach [5]-[7] or the variational approach to fracture [8],[9]. We are rather in the vein of transition from damage to fracture as in [10]. However, the TLS will not be in need of a cohesive zone to perform the transition. The model can be considered as a continuous transition from damage to fracture.

*d*, thus avoiding spurious localization. One imposes that the spatial damage distribution satisfies at all time

*Ω*is the domain of interest. The choice of the function

*f*(

*d*) will be discussed in what follows. As damage evolves, one eventually wants to locate the crack, i.e. the zone for which

*d*=1. However, finding the iso-contour

*d*=1 for a quantity

*d*than cannot go beyond 1 is a tedious operation. This is where the level set ingredient comes into play. Variable

*d*is expressed in terms of a level set

*ϕ*as depicted in Figure 1. This relation introduces a length scale

*l*

_{c}. Finding the zone

*d*=1, is now well-posed since the level set

*ϕ*is not strictly limited to

*l*

_{c}but may go beyond. With the use of the surrogate variable

*ϕ*, condition (1) may be rewritten as

*f*(

*d*) in (1) is related to

*d*(

*ϕ*) by

*f*(

*d*)=

*d*

^{′}(

*ϕ*(

*d*)) (the prime indicating the derivative of

*d*with respect to

*ϕ*). The function

*d*(

*ϕ*) is called the damage shape function and is the main ingredient of the TLS. Equation (2) above indicates that

*ϕ*is a distance function in the zone where the constraint is active (we name this zone the localization zone). The evolution of a distance function has been analyzed and updating algorithm proposed in [11]. In the localization zone, the evolution of

*ϕ*is non-local, indeed

*ϕ*is thus uniform on any segment aligned with ∇

*ϕ*and the rate of

*d*is given by $\stackrel{.}{d}={d}^{\prime}\left(\varphi \right)\stackrel{.}{\varphi}$. Such segments over which $\stackrel{.}{\varphi}$ is uniform are depicted in Figure 2. In the local zone, the evolution of

*ϕ*stems from the evolution of

*d*and the relation

*d*=

*d*(

*ϕ*).

The delocalization (1) used in the TLS is different from existing delocalization techniques. Indeed, it directly uses the norm of the damage gradient. It is thus a Hamilton-Jacobi type equation. On the contrary, damage gradient models [12]-[14] yield Laplacian damage type equation rising the question of proper boundary conditions.

The TLS shares some similarities with the so-called non-local integral approach [15],[16] in which weighted averages are performed over segments (1D), disks (2D) and spheres (3D) of fixed size. In the TLS approach, however, weighted averages are always performed on segments (Figure 2) whatever the dimension of the body and over a length which is not fixed in time but evolves from zero to a maximum length *l*_{c}. Finally, note that as *l*_{c} is the minimal distance between a point where *d*=0 and a fully damaged point, *d*=1, it plays the role of the fracture process zone size.

After this quick introduction of the TLS, we get to the objective of the paper. In previous TLS paper, the delocalization condition (2) was considered as an equality on the whole domain. It meant that *d* was zero on the domain except in zone where the gradient norm was fixed. The short-coming of this view was that uniform or smooth damage field (because of damage hardening for instance) could not be modeled prior to localization. The inequality analyzed in this paper allows a combination of local and non-local evolutions. In the literature, the possibility to combine both local and non-local approach is seldom discussed with the exception of the so-called morphing numerical technique [17],[18].

The paper is organized as follows. The TLS concept with the inequality constraint discussed above are detailed in the first section. Next, the TLS boundary value problem is set up and a dissipation analysis is carried out. A 1D pull-out is solved semi-analytically to show the main feature of the TLS solution. This 1D test is then solved numerically with the TLS to observe the influence of the parameters choice in the model. A conclusion and perspectives end the paper.

## Methods

We consider a solid body occupying a domain *Ω*. The external surface *∂* *Ω* is composed of two parts *∂Ω* *u*_{
u
} and *∂Ω* *u*_{
T
} on which the displacements *λ* u^{d} and the loading *λ* T^{d} are prescribed, respectively. The parameter *λ* is a loading parameter.

Small strains and displacements are assumed as well as quasi-static evolution. The current state is characterized by the displacement field u, from which the strain field $\mathit{\mathbf{\epsilon}}=\frac{1}{2}(\nabla \mathit{u}+\nabla {\mathit{u}}^{T})$ is derived. The current state is also characterized by an internal scalar variable, the damage denoted *d*. In this paper, we will not consider other internal variables.

*ψ*(𝛜,

*d*) from which the stress tensor σ and local energy release rate

*Y*may be derived

The potential *ψ* is assumed for now at least convex with respect to 𝛜. The need for other properties will be discussed later.

*y*depending on damage and strain history (through

*e*) such that

*Y*

_{c}is some threshold. We believe the above formalism encompasses most of the damage models in the literature. To be even more general, one may consider two relations of the kind (5): one for damage in tension and a second one for damage in compression and then combine these damages into

*d*. One has a so-called associated damage model when the

*y*variable is

*Y*. In this case, damage evolution is expressed in terms of the dissipation potential

*φ*

^{*}(

*Y*) which is the indicator function of

*Y*−

*Y*

_{c}≤0:

Such model was already considered in [1] for dissymmetric tension-compression evolution. We emphasize the fact that the TLS description is not restricted to associated damage models.

*d*=1. Numerically speaking, finding the set of points for which

*d*=1 knowing that

*d*may not go beyond 1 is not very practical. This is why the TLS expresses damage in terms of a surrogate variable

*ϕ*whose values are not limited as depicted in Figure 1. We assume the following regularity on

*d*(

*ϕ*)

Finding the subdomain where *d*=1 is equivalent to find the subdomain whose boundary is the iso-contour *ϕ*=*l*_{c}.

*f*(

*d*) is given by

*d*is linear with respect to

*ϕ*, the gradient of damage will be bounded by a constant

*d*(

*ϕ*), the bound depends on the level of damage. For instance, for the profile shown in Figure 1, we have

*n*≥1, we obtain

*t*, the domain may thus be decomposed into three non-overlapping zones : a local zone

*Ω*

^{−}, a non-local zone

*Ω*

^{+}and a fully damaged zone

*Ω*

_{c}

*Γ*

_{c}of the fully damaged zone and the interface

*Γ*between the local and non-local zones.

The boundary *Γ*_{c} defines the crack faces. Figure 2 shows a typical scenario of a crack appearing inside the localization zone.

Note that the volume measure of *Ω*_{c} may be zero. This information is part of the solution process. We expect different shapes of *Ω*_{c} in comminution and brittle crack propagation.

### Eikonal equation

*ϕ*(x)║=1 is a non-linear first-order partial differential equation. It is called an eikonal equation and belongs to the Hamilton-Jacobi equation family. Among the possible solution satisfying ║∇

*ϕ*(x)║=1, we will pick the one corresponding to the vanishing viscosity solution [19]. It is characterized by

*d*(x,y) is the length of the shortest path connecting x and y inside

*Ω*

^{+}. The value of

*ϕ*at x∈

*Ω*

^{+}can be thought as the minimal fare to go from

*Γ*to x. The fare being the sum of the initial fare

*ϕ*(y) plus the mileage from y to x. Damage on

*Ω*

^{+}is thus fully determined from values on

*Γ*. A 1D example of

*ϕ*satisfying the eikonal on a segment [

*b*,

*d*] is given in Figure 3.

The fact that damage is related to a variable satisfying the eikonal equation, the cornerstone of the level set technology [11], explains why the damage model is coined Thick Level Set. In the non-local zone, damage is modeled over a thick layer in terms of level sets.

### Damage evolution

*Ω*

^{−}, damage evolution is local and given by (5). In the non-local zone,

*Ω*

^{+}, damage rate is related to $\stackrel{.}{\varphi}$ by

*ϕ*, see Equation (3). We denote this space as $\mathcal{A}$:

Non-local damage evolution boils down to decomposing *Ω*^{+} into a set of independent segments and finding a value $\stackrel{.}{\varphi}$ over each of them.

The above indicates that duality is preserved through the averaging technique. This is not often the case in delocalization techniques as discussed in [20].

*Y*

_{c}uniform (if not it needs to be averaged by formula (25)). Finally, we write the relation giving $\stackrel{.}{\varphi}$ in terms of $\stackrel{\u2013}{\stackrel{.}{d}}$:

### TLS boundary value problem

The fact that the fully damage zones are removed from the domain is important. It allows the displacement to be discontinuous across *Γ*_{c}. Regarding the regularity of the displacement, we request that the energy, i.e. integral of *ψ* over *Ω*\*Ω*_{c}, is finite. This space is not simply *H*^{1} as in elasticity since the stiffness is possibly vanishing on *Γ*_{c} boundary [21].

*ϕ*variable, it is required to be continuous over

*Ω*and belong to the set . The admissible set for

*ϕ*is denoted K.

*ϕ*leads to a Hadamard compatibility condition on the moving boundary

*Γ*. Let us define the jump of a quantity

*f*across

*Γ*by

*f*defined at x on

*Γ*has the following meaning

*Ω*

^{+}. With these notations we have

where *v*_{n} is the normal velocity of *Γ* counted positively along n. This gives the respective evolution of domains *Ω*^{+} and *Ω*^{−}.

Note that the same free energy expression, *ψ*, is used over *Ω*^{+} and *Ω*^{−}. In what follows, n is the outward normal vector to *Ω* on *∂* *Ω* and to *Ω*^{+} on *∂* *Ω*^{+}. The set of admissible displacements variations is denoted as ${\mathcal{U}}_{0}$. It has the same definition as except that u is set to zero on *∂* *Ω*_{
u
}.

*t*, the spatial distribution of

*ϕ*of the two volumes

*Ω*

^{+}and

*Ω*

^{−}is known, the displacement field u is the field that solves the stationarity of the potential energy:

*Γ*

_{c}is traction free (no contact on crack faces). The equilibrium (39) yields the following local equations

*Γ*

_{c}denotes the boundary of the fully damage zone and thus in case of a crack

*Γ*

_{c}indicates

*both*crack lips. To complete the set of equations to be solved for a known damage distribution, we add the stress definition and kinematic relations

Finally, we need to add damage evolution equations in the local zone (5) and non-local zone (28).

### Dissipation analysis and fields regularity

The goal of this section is to analyze the expression of the dissipation as well as looking at the fields regularity across the boundary *Γ*.

In the above, we did not consider the energy inside *Ω*_{c} because it is assumed to be zero. Indeed, no compression is considered in this zone (see (43)).

*Γ*, that is the displacement jump across

*Γ*must be zero at all time. As a consequence, the derivative along the moving interface of the displacement jump must be zero, [22], yielding the so called first Hadamard compatibility condition between the front velocity

*v*

_{n}and the jump in material velocities ${\left[\stackrel{.}{\mathit{u}}\right]}_{\Gamma}$:

The first term is the dissipation created by the interface propagation. We show now that due to damage continuity on *Γ* this term is zero.

*Γ*, the product of the jump in stress and strain across

*Γ*is zero, [23],[24]:

*ψ*

_{d}(ϵ) be the density of free energy for a given value of damage and let ${\psi}_{\mathrm{d}}^{*}\left(\mathit{\sigma}\right)$ be its dual by the Legendre-Fenchel transform. Since the couples (ϵ

^{+},σ

^{+}) and (ϵ

^{−},ϵ

^{−}) do satisfy the constitutive model (4), we have

^{+},σ

^{−}) and (ϵ

^{−},σ

^{+}) do satisfy the constitutive model. Assuming that the convex potential

*ψ*

_{d}(ϵ) is such that the stress associated to any strain is unique, we have

*Γ*leads to the continuity of the displacement gradient

The dissipation must be positive. For classical models in which *Y* is positive, this implies that damage may only grow. Damage growth will create a growth of the fully damaged zone *Ω*_{c} (and thus a negative velocity *v*_{n}). The last term in (62) is thus automatically positive. Whether this term is zero or not depends on the regularity of *ψ* on the boundary *Γ*_{c}. This regularity must be assessed from the non-local constitutive model condition: $\stackrel{-}{y}-{Y}_{\mathrm{c}}\le 0$.

where $\stackrel{-}{Y}$ is defined by (25) (*y* replaced by *Y*). The above expression exhibits the duality between $\stackrel{-}{Y}$ and $\stackrel{-}{\stackrel{.}{d}}$ in the localization zone.

## Results

*r*

_{ i }is considered rigid and infinitely long. It is pulled out of a clamped circular domain of radius

*r*

_{ e }=

*r*

_{ i }+

*L*. The only non-zero stress component is the shear stress

*τ*satisfying the following equilibrium conditions

*h*(

*d*), satisfying

*h*(1)=0. The shear stiffness is denoted

*μ*and

*Y*

_{c}is also a material parameter.

*Y*=

*Y*

_{c}reduces to

*g*(

*d*) we will be considering. Basically, we are interested by

*C*

^{1}positive concave functions with a maximum value at some damage

*d*

_{c}<1 :

*T*needed to move by a (non-dimensional) displacement

*U*the fiber:

### Pure elastic regime: T∈ [ 0,TA=1]

### Local damage regime: T∈ [ 1,TB]

*T*reaches 1 local damage starts around the fiber. Its distribution is obtained by combining (64) and (69)

*r*=

*r*

_{ i }and of value

*d*

_{ i }=

*d*(

*r*

_{ i }). Considering a general power law damage profile (13), the condition (76) is

*T*

_{ B }the corresponding loading. Due to the fact that

*g*

^{′}(

*d*

_{c})=0, it is clear that ${d}_{i}^{B}$ will be slightly lower than

*d*

_{c}. We note that as the material length gets bigger with respect to

*r*

_{ i }, non-locality (violation of (78)) will step in for smaller and smaller damage

*d*

_{ i }. Considering the choice (71), we get the condition

*n*=1, we get

As a numerical application, with *d*_{c}=0.5 and *l*_{c}/*r*_{
i
}=0.1, we get ${d}_{i}^{B}=0.47$.

### Combined local and non-local damage regime: T∈ [ TB,TC]

*T*

_{ B }, non-local damage will develop close to the fiber. Let [

*r*

_{ i },

*r*

_{ l }] be the current extension of the non-local damage zone in which damage ranges from

*d*

_{ i }to

*d*

_{ l }following:

*d*

_{ l }damage at

*r*=

*r*

_{ l }, following

Given *T*, system (84)-(85) returns unknowns *d*_{
i
} and *d*_{
l
} as well as the extent of the non-local zone *r*_{
l
}=*r*(*d*_{
l
},*d*_{
i
}). We note that for *T*=*T*_{
B
}, we have *d*_{
l
}=*d*_{
i
} and *r*_{
l
}=*r*_{
i
}. Let *T*_{
C
} be the loading above which the system has no solution.

### Non-local damage regime: T decreases from TCto 0

*T*

_{ C }. When the loading decreases below

*T*

_{ C }, there is of course a possible elastic solution. Another possible solution is the further development of the non-local damage zone (while damage in the local zone no longer evolves since loading is decreasing). The system of equations to solve still involves (84)

Indeed the damage at *r*_{
l
} did not change from its value at load *T*_{
C
} because the load has been decreasing afterwards.

### Analysis of the displacement of the fiber

*d*(

*ϕ*). Going back to the displacement expression, (88), we have

*C*is a finite constant and

*ϕ*(

*d*) as

*d*goes to 1:

When *n*<2, the fiber displacement must be zero for total failure. When *n*=2, there exists a limit value of fiber displacement before total failure and when *n*>2, it takes an infinite displacement before total failure. It is interesting to note that these three regimes also exist in gradient damage models [20].

### Numerical solve

Last section gave some insight on the different regimes in the solution. In order to plot the solution, we detail here a 1D numerical solver. This code is rather ad hoc for 1D problem, since we force the advance of the *Γ* boundary and find the corresponding loading and fields. General 2D and 3D solvers will be detailed in a forthcoming paper. We search for the solution at a set of discrete times. Consider the solution known at time *t*_{
n
}, the solution at time *t*_{n+1} must satisfy the following equations.

**Kinematics and equilibrium on ]**r

_{ i }

**,**r

_{ e }

**[.**

**State laws and**d

**(**ϕ

**) relation on ]**r

_{ i }

**,**r

_{ e }

**[.**

**Non-local evolution law on**$]{r}_{i},{r}_{l}^{n+1}[$

**.**

**Local evolution law on**$]{r}_{l}^{n+1},{r}_{e}[$

**.**

Regarding space discretization, the segment ]*r*_{
i
},*r*_{
e
}[ is discretized with a set of finite elements. Initially, the non-local zone is empty and we proceed with a classical Newton-Raphson scheme depicted in the solver flowchart without non-local zone.

**Solver flowchart without non-local zone**

- 1.
initialization:

*u*^{0}=*d*^{0}=*T*^{0}=0 - 2.
elastic step: find the load step for which damage starts

- 3.
load step

*T*^{n+1}=*T*^{ n }+*Δ**T* - 4.
iterations initialization

*k*=0 - 5.
solve linear system (110) to find

*Δ**u* - 6.
after the first iteration adapt the load step so that the maximum damage increment is

*d*_{inc} - 7.
- 8.
if residual ≤ tol, go to 9 else go to 5

- 9.
if ║∇

*ϕ*^{n+1}║≤1, go to 3, else go to solver flowchart with non-local zone

*k*. Once the displacement correction is obtained, the local update of the fields is computed from

At the end of each load step, the gradient of the level set is computed. If it is below 1 everywhere the next load step is applied. If not, a non-local zone is placed and the solver flowchart with non-local zone is used.

**Solver flowchart with non-local zone**

- 1.
initialization: ${r}_{l}^{0}={r}_{i}$

- 2.
increase non-local zone: ${r}_{l}^{n+1}={r}_{l}^{n}+\Delta {r}_{l}$

- 3.
iterations initialization:

*k*=0 - 4.
linear solve: solve (119) to find

*Δ**u*,*Δ**T*,*Δ**ϕ* - 5.
load update:

*T*^{k+1}=*T*^{ k }+*Δ**T* - 6.
- 7.
if residual ≤ tol, go to 8, else go to 4

- 8.
if domain not fully broken (

*d*(*r*_{ i })<1), go to 2, else go to 9 - 9.
end

The extent of the non-local zone is imposed and one tries to find a continuous displacement and damage field satisfying the problem.

*η*

^{ k }is evaluated following (116). The update in the local zone follows (111)-(118) whereas in the non-local zone we have

Is is interesting to note the difference between the two solver flowcharts. When the non-local zone is empty, the linear solve deals only with displacement increments and the local update deals with the damage variable. On the contrary, when the non-local zone is not empty, the linear solve involves both displacement and damage (or more precisely the surrogate *ϕ* variable) increment in the non-local zone (local zone being treated as before).

*j*is located at a position

*x*(

*j*) given by

*N*is the number of elements considered. Results will be shown for the following mechanical parameters:

*Δ*

*r*

_{ l }, the non-local zone is advanced by one element at a time or smaller when damage gets close to 1 at

*r*

_{ i }. This is done in order to capture the full load-displacement curve. The formula used in the simulation is

where *h*^{*} is the size of the element adjacent to the non-local zone at time step *n*. The initial (*n*=0) non-local zone needs to be more than one-element for convergence. Between 5 and 10 elements are used.

As a final remark on the solver flowchart with the non-local zone, we noticed that in non-local zone update, it was more efficient (reduced number of iterations) to take *Δ* *ϕ* as the one ensuring damage continuity rather that picking the one coming from step 3.

## Discussion

*ϕ*and damage along the radius at different loads are depicted in Figure 7.

*n*. Plots confirm the analytical limit results (97). As long as damage is purely local, all curves are superposed. As non-locality steps in, the delocalization parameters

*n*plays a role.

*N*,

*d*

_{inc}, we show Figure 9 the influence of the choice of the

*N*parameter (for the case

*n*=2 and

*d*

_{inc}=0.02). In Figure 10, we show the influence of

*d*

_{inc}(for the case

*n*=2 and

*N*=50). Note that as expected, parameter

*d*

_{inc}has only an influence when damage is purely local (rising part of the curve). For both figures, a zoom was used. Otherwise, curves cannot be distinguished.

## Conclusions

The Thick Level Set damage model allows coupling local damage evolution in some part of the domain to a non-local damage evolution in the localization zone. Damage gradient is bounded. The bound is reached in the non-local zone (localization zone) and not reached in the local one. The localization zone boundary is the main unknown in the model. It evolves ensuring damage continuity. A semi-analytical 1D solution has been developed showing different regimes in the solution (elastic, local damage, coupled local and non-local damage and finally pure non-local damage). The solution was plotted using a numerical scheme. This numerical scheme is ad hoc for the 1D problem considered. The corresponding numerical implementation for 2D and 3D cases will be the subject of a forthcoming publication.

## Authors’ contributions

All authors contributed to the main ideas in the paper: the way to couple local and non-local evolutions of damage. NM came up with the analytical solution. NM and NC designed the 1D code to plot the results. All authors read and approved the final manuscript.

## Declarations

### Acknowledgements

The support of the ERC Advanced Grant XLS no 291102 is greatfully acknowledged. Professor Antonio Huerta is also acknowledged for his advice.

## Authors’ Affiliations

## References

- Moës N, Stolz C, Bernard P-E, Chevaugeon N:
**A level set based model for damage growth: the thick level set approach.***Int J Numer Meth Eng*2011,**86:**358–380. 10.1002/nme.3069View ArticleGoogle Scholar - Bernard P-E, Moës N, Chevaugeon N:
**Damage growth modeling using the Thick Level Set (TLS) approach: efficient discretization for quasi-static loadings.***Comput Meth Appl Mech Eng*2012,**233–236:**11–27. 10.1016/j.cma.2012.02.020View ArticleGoogle Scholar - Stolz C, Moës N:
**A new model of damage: a moving thick layer approach.***Int J Fract*2012,**174:**49–60. 10.1007/s10704-012-9693-3View ArticleGoogle Scholar - Stolz C, Moës N:
**On the rate boundary value problem for damage modelization by Thick Level Set.***ACOME 2012 Proceeding*Ho-Chi-Minh, Viet Nam; 2012. [http://hal.archives-ouvertes.fr/hal-00725635] http://hal.archives-ouvertes.fr/hal-00725635 http://hal.archives-ouvertes.fr/hal-00725635Google Scholar - Karma A, Kessler D, Levine H:
**Phase-field model of mode III dynamic fracture.***Phys Rev Lett*2001,**87**(4):045501. 10.1103/PhysRevLett.87.045501View ArticleGoogle Scholar - Miehe C, Welschinger F, Hofacker M:
**Thermodynamically consistent phase-field models of fracture: Variational principles and multi-field FE implementations.***Int J Numer Meth Eng*2010,**83**(10):1273–1311. 10.1002/nme.2861MathSciNetView ArticleGoogle Scholar - Spatschek R, Brener E, Karma A:
**Phase field modeling of crack propagation.***Phil Mag*2011,**91**(1):75–95. 10.1080/14786431003773015View ArticleGoogle Scholar - Francfort GA, Marigo J-J:
**Revisiting brittle fracture as an energy minimization problem.***J Mech Phys Solid*1998,**46:**1319–1412. 10.1016/S0022-5096(98)00034-9MathSciNetView ArticleGoogle Scholar - Bourdin B, Francfort GA, Marigo J-J (2008) The Variational Approach to Fracture, 5–148, , [http://link.springer.com/10.1007/s10659-007-9107-3] Bourdin B, Francfort GA, Marigo J-J (2008) The Variational Approach to Fracture, 5–148,
- Comi C, Mariani S, Perego U:
**An extended FE strategy for transition from continuum damage to mode I cohesive crack propagation.***Int. J. Numer. Anal. Meth. Geomech*2007,**31:**213–238. 10.1002/nag.537View ArticleGoogle Scholar - Sethian JA:
*Level set methods and fast marching methods: evolving interfaces in computational geometry, fluid mechanics, computer vision and material science*. Cambridge University Press, UK; 1999.Google Scholar - Maugin GA:
**Internal variables and dissipative structures.***J Non-Equilibrium Therm*1990,**15:**173–192.Google Scholar - Frémond M, Nedjar B:
**Damage, gradient of damage and principle of virtual power.***Int J Solid Struct*1996,**33**(8):1083–1103. 10.1016/0020-7683(95)00074-7View ArticleGoogle Scholar - Comi C:
**Computational modelling of gradient-enhanced damage in quasi-brittle materials.***Mech Cohesive-Frictional Mater*1999,**36**(April 1997):17–36. 10.1002/(SICI)1099-1484(199901)4:1<17::AID-CFM55>3.0.CO;2-6View ArticleGoogle Scholar - Pijaudier-Cabot G, Bazant ZP:
**Nonlocal dalmage theory.***J Eng Mech ASCE*1987,**113:**1512–1533. 10.1061/(ASCE)0733-9399(1987)113:10(1512)View ArticleGoogle Scholar - Bazant ZP, Jirasek M:
**Nonlocal integral formulations of plasticity and damage: survey of progress.***J Eng Mech*2002,**128**(November):1119–1149. 10.1061/(ASCE)0733-9399(2002)128:11(1119)View ArticleGoogle Scholar - Lubineau G, Azdoud Y, Han F, Rey C, Askari A:
**A morphing strategy to couple non-local to local continuum mechanics.***J Mech Phys Solid*2012,**60**(6):1088–1102. 10.1016/j.jmps.2012.02.009MathSciNetView ArticleGoogle Scholar - Azdoud Y, Han F, Lubineau G:
**A Morphing framework to couple non-local and local anisotropic continua.***Int J Solid Struct*2013,**50**(9):1332–1341. 10.1016/j.ijsolstr.2013.01.016View ArticleGoogle Scholar - Lions P-L:
*Generalized solutions of Hamilton-Jacobi equations*. Pitman Advanced Publishing Program, Boston; 1982.Google Scholar - Lorentz E, Godard V:
**Gradient damage models: toward full-scale computations.***Comput Meth Appl Mech Eng*2011,**200**(21–22):1927–1944. 10.1016/j.cma.2010.06.025MathSciNetView ArticleGoogle Scholar - Chung-Min L, Rubinstein J:
**Elliptic equations with diffusion coefficient vanishing at the boundary: theoretical and computational aspects.***Quaterly Appl Math*2006,**64:**725–747.Google Scholar - Pradeilles-Duval RM, Stolz C:
**Mechanical transformations and discontinuities along a moving surface.***J Mech Phys Solid*1995,**43**(1):91–121. 10.1016/0022-5096(94)00061-9MathSciNetView ArticleGoogle Scholar - Hill R:
**Energy-momentum tensors in elastostatics: some reflections on the general theory.***J. Mech. Phys. Solids*1986,**34**(3):305–317. 10.1016/0022-5096(86)90022-0MathSciNetView ArticleGoogle Scholar - Stolz C:
**On micro-macro transition in non-linear mechanics.***Materials*2010,**3**(1):296–317. 10.3390/ma3010296View ArticleGoogle Scholar - Rockafellar RT:
*Convex analysis*. Princeton University Press, USA; 1970.View ArticleGoogle Scholar

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.